Material Testing of Coated Alloys in a Syngas Combustion Environment Year 6 - Activity 1.13 - Development of a National Center for Hydrogen Technology [electronic resource].
- Washington, D.C. : United States. Dept. of Energy, 2011.
Oak Ridge, Tenn. : Distributed by the Office of Scientific and Technical Information, U.S. Dept. of Energy.
- Additional Creators:
- University of North Dakota
United States. Department of Energy
United States. Department of Energy. Office of Scientific and Technical Information
- Modifications were made to the inlet of the existing Energy & Environmental Research Center (EERC) thermal oxidizer to accommodate side-by-side coupon holders for exposure testing. Two 5-day tests with over 200 hours of total exposure time were completed. The first week of testing was conducted in enriched air-blown mode, with coupon temperatures ranging from 128° to 272°F. Carbonyl sampling was conducted, but it was discovered after the fact that the methodology used was producing very low recoveries of iron and nickel carbonyl. Therefore, the data generated during this week of testing were not considered accurate. The second week of testing was conducted in oxygen-blown mode, with coupon temperatures ranging from 220° to 265°F. Two improved methods were used to measure carbonyl concentration during this week of testing. These methods produced results closer to equilibrium calculations. Since both weeks of testing mostly produced a product gas with approximately 15%–18% carbon monoxide, it was felt that actual carbonyl concentrations for Week 1 should be very similar to those measured during Week 2. The revised carbonyl sampling methodology used during the second week of testing greatly improved the recovery of iron and nickel carbonyl in the sample. Even though the sampling results obtained from the first week were inaccurate, the results from the second week can be used as an estimate for the periods during which the gasifier was operating under similar conditions and producing similar product gas compositions. Specifically, Test Periods 2 and 3 from the first week were similar to the conditions run during the second week. For a product gas containing roughly 15%–18% CO and a coupon temperature of approximately 220°–270°F, the nickel carbonyl concentration should be about 0.05–0.1 ppm and the iron carbonyl concentration should be about 0.1–0.4 ppm. After each week of testing the coupons were recovered from the coupon holder, weighed, and shipped back to Siemens for analysis.
- Published through SciTech Connect.
- Type of Report and Period Covered Note:
- Funding Information:
View MARC record | catkey: 14102419